Download presentation

Presentation is loading. Please wait.

Published byYuliana Witcraft Modified over 2 years ago

1
Adsorption and Catalysis Dr. King Lun Yeung Department of Chemical Engineering Hong Kong University of Science and Technology CENG 511 Lecture 3

2
Physical Adsorption Texture and morphology –specific surface area of catalyst –pore size –pore shape –pore-size distribution (same size or various sizes?) –pore volume

3
Pore Size and Shape Pore Diameter –micropores (< 2 nm) –mesopores (2 – 50 nm) –macropores (> 50 nm) Pore Shape –cylinder –slit –ink-bottle –wedge

4
Pore Size and Shape Pore Structure Silica Carbon Zeolite

5
Pore Size and Shape Why is it important? it dictates the diffusion process through the material.

6
Pore Size and Shape Why is it important? directly affect the selectivity of the catalytic reaction.

7
Pore Size and Shape Measurement Techniques 1 10 100 1000 10000 Pore diameter (nm) Micro Meso Macro 2 50 N 2 capillary condensation Hgporosimetry

8
N 2 Physisorption Adsorption and Desorption Isotherms Adsorption Desorption

9
Adsorption and Desorption Isotherms III n ad p / p 0 VI n ad p / p 0 V n p / p 0 I n p / p 0 p / p II n ad 0 B IV n ad p / p 0 B N 2 Physisorption

10
Isotherms Assumptions: homogeneous surface (all adsorption sites energetically identical) monolayer adsorption (so no multilayer adsorption) no interaction between adsorbed molecules I n ad p / p 0 Type I Langmuir Adsorption Isotherm

11
Isotherms Multilayer adsorption (starting at B) Common for pore-free materials p / p n ad 0 B Type II Type IV Similar to II at low p Pore condensation at high p n ad p / p 0 B

12
Isotherms Type III Type IV n ad p / p 0 Strong cohesion force between adsorbed molecules, e.g. when water adsorbs on hydrophobic activated carbon n ad p / p 0 Similar to III at low p Pore condensation at high p

13
Physisorption Surface area measurement

14
Physisorption Different Adsorbates Used in Physisorption Studies

15
N 2 Physisorption Adsorption and Desorption Isotherms Langmuir Adsorption? No: strong adsorption at low p due to condensation in micropores at higher p saturation due to finite (micro)pore volume

16
BET Isotherm

18
Nonporous Silica and Alumina Low p/p 0 : filling of micropores favoured adsorption at most reactive sites (heterogeneity) High p/p 0 : capillary condensation Range 0.05 < p/p 0 < 0.3 is used to determine S BET BET equation

19
Pore Size and Surface Area

20
Pore Size Distribution Kelvin Equation

21
Pore Size Distribution Kelvin Equation Cylindrical pore Ink-bottle pore Pore with shape of interstice between close-packed particles Adsorbed layer t dpdp dmdm

22
Kelvin Equation

23
Pore filling Model Cylindrical Pore Channel

24
Hysteresis Loop Information on pore shape

25
Pore Size Distribution t-Method n ad t Proportional to S t Note: n ad is experimental result t is calculated from correlation t versus p

26
Kelvin Equation t-Method

27
Kelvin Equation Shape of t-plots

28
Kelvin Equation Interpretation of t-Plot -alumina

29
Kelvin Equation Pore Size Distribution -alumina r = t + 2 V RTIn P0P0 P

30
Mercury Porosimetry Pore Size Distribution

31
Mercury Porosimetry Pore Size Distribution -alumina

32
N 2 Physisorption versus Hg Porosimetry Hg cannot penetrate small (micro)pores, N 2 can Uncertainty of contact angle and surface tension values Cracking or deforming of samples

33
Texture Data on Common Catalysts

34
N 2 Adsorption Isotherms & Pore Volume Distributions wide-pore silica -alumina N 2 Adsorption Isotherms & Pore Volume Distributions

35
-alumina activated carbon

36
Raney NiZSM-5 N 2 Adsorption Isotherms & Pore Volume Distributions

37
wide-pore silica -alumina Hg Intrusion Curves & Pore Volume Distributions

38
-alumina activated carbon

39
Raney NiZSM-5 Hg Intrusion Curves & Pore Volume Distributions

40
BET- & t-plots wide-pore silica -alumina

41
-alumina activated carbon BET- & t-plots

42
Raney NiZSM-5 BET- & t-plots

43
Chemisorption Surface Characterization Specific surface area of phases Types of active sites Number of active sites Reactivity of active sites Stability of active sites

44
Chemisorption Metal Dispersion

45
Adsorption Mode

46
Adsorption Stoichiometry

47
Particle Size and Dispersion

48
Supported Metal Particles

49
Number of Surface Atoms

50
Pulse Chemisorption

51
Monolayer capacity: 0.06 mmol / g Pt On-line Thermoconductivity Detector

52
Step Chemisorption On-line Mass Spectrometer

53
Temperature Programmed Desorption Adsorption Site Differentiation NH 3 desorption from HZSM-5

54
Temperature Programmed Desorption Adsorption Energetics After ammonia saturation the sample is degassed at 120 °C for 60 minutes Heating Rate of 5, 10, 15 and 20 °C/min

55
Temperature Programmed Desorption Adsorption Energetics Beta = heating rate [K / min] Tp = maximum desorption peak temperature Ed = Desorption energy [Kj / mole] A = Arrhenius factor R = 8.314451 [J / mol K] 12.49A factor 24.51Ed (kJ/mole) 5.4639Intercept 2948.07Slope

56
Temperature Programmed Reduction –characterisation of oxidic catalysts and other reducible catalysts –qualitative information on oxidation state –quantitative kinetic data –optimisation of catalyst pretreatment

57
Temperature Programmed Reduction Fe 2 O 3

58
Temperature Programmed Reduction Fe 2 O 3 Dry H 2 /Ar

59
Wet H 2 /Ar (3% H 2 O) Temperature Programmed Reduction Fe 2 O 3

60
Temperature Programmed Reduction Fe 2 O 3

61
Kinetic Models for Reduction

62
Infrared Spectroscopy

63
Reactor Cell DRIFTS Transmittance

64
Analysis of Catalyst Preparation Surface Hydroxyl Groups NH 4 ReO 4 Alumina Dry impregnation Drying 383 K, 16 h Calcination 323 K, 2 h Re 2 O 7 / Alumina

65
Analysis of Catalyst Preparation

66
IR Probe Molecule Acidity Measurement

67
IR Probe Molecule Acidity Measurement

68
Kelvin Equation Pore Size Distribution

69
Kelvin Equation Pore Size Distribution

70
In-Situ Reaction Study TCE Photocatalytic Oxidation

71
In-Situ Reaction Study PCO of Ethylene

72
In-Situ Reaction Study PCO of 1,1-DCE

73
In-Situ Reaction Study PCO of cis-1,2-DCE

74
In-Situ Reaction Study PCO of trans-1,2-DCE

75
In-Situ Reaction Study PCO of TCE

76
In-Situ Reaction Study PCO of Tetrachloroethylene

Similar presentations

OK

Experimental Methods in Catalysis (EMC) M.Tech-Catalysis Technology II Semester CT-503 Dr.K.R.Krishnamurthy National Centre for Catalysis Research Indian.

Experimental Methods in Catalysis (EMC) M.Tech-Catalysis Technology II Semester CT-503 Dr.K.R.Krishnamurthy National Centre for Catalysis Research Indian.

© 2018 SlidePlayer.com Inc.

All rights reserved.

Ads by Google

Ppt on odisha culture Download ppt on transportation in animals and plants Ppt on preservation of public property definition Ppt on self development academy How to make a ppt on a mac Perspective view ppt on iphone Ppt on grease lubrication pump Ppt on presentation skills communication 3d backgrounds for ppt on social media Ppt on project management training